Caught in Action. The Late Rare Earths Thulium and Lutetium Substituting Aluminum Atoms in the Structure of Ca14AlBi11
Baranets, Sviatoslav; Bobev, Svilen; Journal of the American Chemical Society  (2020) –; doi:10.1021/jacs.0c11026

data_4135468
_publ_section_title
;
 Caught in Action. The Late Rare Earths Thulium and Lutetium Substituting
 Aluminum Atoms in the Structure of Ca14AlBi11
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_paper_doi               10.1021/jacs.0c11026
_journal_year                    2020
_chemical_formula_moiety         'Al0.9 Bi11 Ca13.939 Lu0.161'
_chemical_formula_sum            'Al0.9 Bi11 Ca13.94 Lu0.16'
_chemical_formula_weight         2909.94
_space_group_crystal_system      tetragonal
_space_group_IT_number           142
_space_group_name_Hall           '-I 4bd 2c'
_space_group_name_H-M_alt        'I 41/a c d :2'
_atom_sites_solution_primary     dual
_audit_creation_date             2020-07-19
_audit_creation_method
;
Olex2 1.3
(compiled 2020.06.28 svn.raecde09e for OlexSys, GUI svn.r6132)
;
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   16.9893(12)
_cell_length_b                   16.9893(12)
_cell_length_c                   22.6602(17)
_cell_measurement_reflns_used    4771
_cell_measurement_temperature    200.02
_cell_measurement_theta_max      29.32
_cell_measurement_theta_min      3.39
_cell_volume                     6540.6(8)
_computing_molecular_graphics    'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 1.3 (Dolomanov et al., 2009)'
_computing_structure_refinement  'SHELXL 2018/3 (Sheldrick, 2015)'
_computing_structure_solution    'SHELXT 2018/2 (Sheldrick, 2018)'
_diffrn_ambient_temperature      200.02
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Bruker APEX-II CCD'
_diffrn_measurement_method       '\f and \w scans'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0937
_diffrn_reflns_av_unetI/netI     0.0359
_diffrn_reflns_Laue_measured_fraction_full 1.000
_diffrn_reflns_Laue_measured_fraction_max 1.000
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -20
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -19
_diffrn_reflns_limit_l_max       31
_diffrn_reflns_limit_l_min       -31
_diffrn_reflns_number            54405
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.698
_diffrn_reflns_theta_min         2.398
_diffrn_source_current           30.0
_diffrn_source_power             1.5
_diffrn_source_voltage           50.0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    61.637
_exptl_absorpt_correction_T_max  0.0497
_exptl_absorpt_correction_T_min  0.0139
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
SADABS-2016/2 (Bruker,2016/2) was used for absorption correction.
wR2(int) was 0.1501 before and 0.0688 after correction.
The Ratio of minimum to maximum transmission is 0.2797.
The \l/2 correction factor is Not present.
;
_exptl_crystal_colour            black
_exptl_crystal_colour_primary    black
_exptl_crystal_density_diffrn    5.910
_exptl_crystal_description       block
_exptl_crystal_F_000             9719
_exptl_crystal_size_max          0.122
_exptl_crystal_size_mid          0.11
_exptl_crystal_size_min          0.077
_refine_diff_density_max         1.939
_refine_diff_density_min         -1.837
_refine_diff_density_rms         0.375
_refine_ls_extinction_coef       0.000035(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     'SHELXL-2018/3 (Sheldrick 2018)'
_refine_ls_goodness_of_fit_ref   1.072
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     64
_refine_ls_number_reflns         2330
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.072
_refine_ls_R_factor_all          0.0398
_refine_ls_R_factor_gt           0.0303
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0190P)^2^+227.4371P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0648
_refine_ls_wR_factor_ref         0.0681
_reflns_Friedel_coverage         0.000
_reflns_number_gt                1969
_reflns_number_total             2330
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            ja0c11026_si_001.cif
_cod_data_source_block           mo_svib1543_0m
_cod_original_cell_volume        6540.6(10)
_cod_original_sg_symbol_H-M      'I 41/a c d'
_cod_original_formula_sum        'Al0.90 Bi11 Ca13.94 Lu0.16'
_cod_database_code               4135468
_shelx_shelxl_version_number     2018/3
_shelx_estimated_absorpt_t_max   0.088
_shelx_estimated_absorpt_t_min   0.050
_olex2_refinement_description
;
1. Shared sites
{Al1, Lu2}
{Ca1, Lu1}
2. Uiso/Uaniso restraints and constraints
Uanis(Al1) = Uanis(Lu2)
Uanis(Ca1) = Uanis(Lu1)
3. Others
 Sof(Lu2)=0.25*(1-FVAR(2))
 Sof(Al1)=0.25*FVAR(2)
 Sof(Lu1)=1-FVAR(2)
 Sof(Ca1)=FVAR(2)
;
_shelx_res_checksum              57370
_shelx_hkl_checksum              90440
_olex2_submission_special_instructions 'No special instructions were received'